advertisement

International Journal of Civil Engineering and Technology (IJCIET) Volume 10, Issue 04, April 2019, pp. 133-141, Article ID: IJCIET_10_04_015 Available online at http://www.iaeme.com/ijmet/issues.asp?JType=IJCIET&VType=10&IType=4 ISSN Print: 0976-6308 and ISSN Online: 0976-6316 © IAEME Publication Scopus Indexed THE APPLICATION OF RESPONSE SURFACE METHODS (RSM) TO STUDY THE EFFECT OF PARTIAL PORTLAND CEMENT REPLACEMENT USING SILICA FUME ON THE PROPERTIES OF MORTAR Annisa Rahmatika*, Hariyadi, Jauhar Fajrin Postgraduate Study Program of Civil Engineering, University of Mataram, Jl. Majapahit no. 62, Mataram, NTB, 83125, Indonesia *Corresponding Author ABSTRACT The addition of pozzolan material, such as silica fume in order to improve mortar or concrete quality has been reported in many papers. However, the previous experimental design was only limited to factors that had a significant influence on the response. In addition, the results of the research analysis are only able to determine differences between the levels of factors and show the maximum or minimum response values, limited to the level of factors planned only. Response Surface Method used in the experiment of this study can analyze the problems of several independent variables that affect the response variable. The basic idea of this method is to use experimental design involving statistics to find the optimal value of the effect of adding silica fume as a partial substitute material for mortar to the compressive strength resulted. The design of the experimental proportion in this study was carried out by replacing 20% silica fume in cement as the middle boundary. Furthermore, the proportion of silica fume, cement and sand is reduced in number to the lower limit and added to the upper limit of the experimental design. Conclusions achieved; 1) Analysis using the Response Surface Method shows the optimal composition of mortar mixture obtained by adding 23.6% silica fume to cement, so that the optimal compressive strength test is at 55.8 MPa. 2) The optimal composition can also reduce the absorption of mortar to water, which only absorbs 5.34% water compared to mortar without silica fume which absorbs water up to 8.84%. 3) Addition of silica fume to mortar can increase 1.33% pH of mortar. The pH of the mortar with the addition of silica fume remained in alkaline conditions 9.75. Key words: mortar, silica fume, response surface method, mortar characteristics. http://www.iaeme.com/IJCIET/index.asp 133 [email protected] Annisa Rahmatika, Hariyadi, Jauhar Fajrin Cite this Article: Annisa Rahmatika, Hariyadi, Jauhar Fajrin, The Application of Response Surface Methods (RSM) to Study the Effect of Partial Portland Cement Replacement Using Silica Fume on the Properties of Mortar, International Journal of Civil Engineering and Technology 10(4), 2019, pp. 133-141. http://www.iaeme.com/IJCIET/issues.asp?JType=IJCIET&VType=10&IType=4 1. INTRODUCTION Mortar is a mixture consisting of binder (cement), fine aggregate (sand), water, and other additives, which are used as constituent material in a construction that is both structural and non-structural. Mortar is a porous mixture that cannot be avoided from the entry of aggressive ions which can cause degradation. Mortar as the outermost layer of the wall that is degraded will become cracked and porous. Therefore, in an effort to prevent or reduce the occurrence of damage, what can be done is to make the concrete mixture denser (waterproof) so that it can withstand the effects of destructive acid [1]. Many studies have shown that an increase in compressive strength and reduced permeability in mortars and concrete with the addition of pozzolan material in form of silica fume. Silica fume contains high layers of SiO2 and is a very fine, round and very small diameter of material that is 1/100 times the diameter of cement. It can fill the cavity between particles in the mortar mixture, so that a more impermeable mortar is obtained [2]. Research presents an experimental study on self-compacting concrete (SCC) involving three types of mixtures, the first consisting of a different percentage of fly ash, the second using different percentages of silica fume and the third using a mixture of fly ash and silica fume. The results of this study is the mixtures of 15% silica fume as a substitute for cement resulting in a higher compressive strength compared to the mixture of 30% fly ash [3]. Silica fume also studied with variations of 0, 5, 10 and 20% in concrete mixtures. Testing of compressive strength on concrete specimens aged 7 and 28 days has increased, respectively 38.30 N / mm2, 41.29 N / mm2, 46.76 N / mm2, 47.3 N / mm2, and 44.27 N / mm2. The results of this study indicate that the use of silica fume can increase the strength of concrete. The optimum compressive strength and flexural strength are obtained in the range of 10-15% silica fume replacement [4]. Based on ref [5], study to determine the effect of silica fume on geopolymer concrete, using variations of silica fume as much as 5, 10, 15 and 20% as a partial substitute for cement. Tests were carried out on geopolymer concrete specimens aged 7 and 28 days. As much as 20% silica fume usage as a substitute for some cement, can increase the compressive strength by 9%, tensile strength up to 10% and flexural strength by up to 12%. So far, the results of several studies on the addition of silica fume as a partial substitute for cement, only analyzed the effect of silica fume with simple statistical calculations. A study with an experimental design method is needed, which can take into account the influence of each constituent material (more than one factor) on the response of an experimental mortar mixture. One of the right methods used in experimental design is Response Surface Method. This method can contribute to the influence of two or more factors in an experiment [6]. The analysis using the surface response method resulted in the design of non-combustible bricks with a mixture of 21,034% cement, 28,9651% sand and 50% soil. With the proportion of the design of the constituent materials of the brick, optimal brick compressive strength was obtained at 50.22 kg/cm2[7]. Experimental design modeling on mortar with the addition of silica fume as a partial substitute for cement has never been done before. In this research, an experimental design will be carried out with silica fume as a partial substitute for cement, which aims to obtain the optimum value and know its effect on the physical and mechanical properties of the mortar. http://www.iaeme.com/IJCIET/index.asp 134 [email protected] The Application of Response Surface Methods (RSM) to Study the Effect of Partial Portland Cement Replacement Using Silica Fume on the Properties of Mortar 2. EKSPERIMENTAL PROGRAMS 2.1. Materials The ingredients of the mortar in this study included PPC cement, sand, water and pozzolanic material, silica fume. Comparison of cement:sand in the mortar mixture used is 30:70 [8]. There are three independent variables namely the proportion of sand, the proportion of cement and the proportion of silica fume. The design of the initial mortar composition design will use 20% silica fume as a partial substitute for cement. 2.2. Mix Proportions The research method used in this study is response surface method on Minitab program 17. Before being input into the Minitab, the design of the proportion of sand, the proportion of cement and the proportion of silica fume as much as 20% is determined as the middle level (code 0), then design proportions for the lower level (code -1) and the upper level (code 1) are obtained by reducing and adding the same number of proportions based on the composition at the middle level. The design can be seen in Table 1. The number of draft proportions in Table 1 is then input to the dialog box in the Minitab 17 program, by selecting Stat - DOE - Create response surface design. There are 20 types of sample designs, which are made with replication of 3 times. The experimental design can be seen in Table 2. Table 1 Number of Mortar Mixed Material Design Proportions Factor Silica Cement Sand -1 (gr) 90 300 1200 0 (gr) 120 480 1400 1 (gr) 150 660 1600 Table 2 Design of Response Surface CCD Experiments No. 1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 StdOrder 1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 RunOrder 1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 PtType 1 1 1 1 1 1 1 1 -1 -1 -1 -1 -1 -1 0 0 0 0 0 0 http://www.iaeme.com/IJCIET/index.asp Blocks 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 135 Sand -1 1 -1 1 -1 1 -1 1 -1.6817 1.6817 0 0 0 0 0 0 0 0 0 0 Cement -1 -1 1 1 -1 -1 1 1 0 0 -1.6817 1.6817 0 0 0 0 0 0 0 0 Silica Fume -1 -1 -1 -1 1 1 1 1 0 0 0 0 -1.6817 1.6817 0 0 0 0 0 0 [email protected] Annisa Rahmatika, Hariyadi, Jauhar Fajrin 3. RESULTS AND DISCUSSION 3.1. Compressive Strength Testing the steps and spesification in making sample of mortar that is implemented in this research as directed by reference [9] using a Compressive Testing Machine (CTM) [10]. The results can be seen in Table 3. Table 3. Compressive Strength Test Results No 1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 Design of Experiment (gr) Silica Fume Cement Sand 90 300 1200 150 300 1200 90 660 1200 150 660 1200 90 300 1600 150 300 1600 90 660 1600 150 660 1600 69.57 480 1400 170.43 480 1400 120 177.42 1400 120 782.58 1400 120 480 1063.8 120 480 1736.2 120 480 1400 120 480 1400 120 480 1400 120 480 1400 120 480 1400 120 480 1400 Compressive Strength (MPa) 1 2 3 30.800 30.500 31.200 42.000 43.500 44.400 40.392 39.216 39.500 40.800 41.200 39.500 32.500 33.200 32.800 40.500 41.212 41.500 42.500 44.400 43.500 38.000 38.400 39.500 18.500 18.846 18.077 26.500 27.200 27.600 45.500 46.000 44.800 52.400 51.500 51.200 46.500 47.755 47.500 47.500 49.200 48.500 56.500 56.800 56.500 56.500 56.500 56.078 56.500 56.500 56.500 56.500 56.000 56.500 57.959 57.143 56.500 56.500 56.800 56.500 Table 4. Analysis of the Order Response Surface Regression Model http://www.iaeme.com/IJCIET/index.asp 136 [email protected] The Application of Response Surface Methods (RSM) to Study the Effect of Partial Portland Cement Replacement Using Silica Fume on the Properties of Mortar 3.2. The Second-Order Model Analysis of Variance Test results of compressive strength in table 3 then analyzed using Response Surface Design in the Minitab 17 program, by selecting Stat - DOE - Response Surface - Analyze Response Surface Design, click Term and select the quadratic model. Quadratic experimental design is used to determine whether the input variable in the compressive strength data has a significant effect or not. Data processing in experiment stage II obtained results as shown in Table 4. As it can be seen in table 4, it is known that the P value obtained is smaller than the value of α (pvalue <α) = 0.05. This indicates that the independent variable contributes significantly to the model formed. The Lack of Fit test results are significant, which is indicated by (pvalue> α) = 0.139 so that the hypothesis H0 is accepted, meaning that there is a suitability of the model or there is no incompatibility of the analysis model. 3.3. Testing the Experimental Model 3.3.1. Identical Test Testing of identical assumptions aims to examine whether the residual variance of the model obtained is the same as the spread. In Figure 1 below, residuals are scattered randomly and do not form a certain pattern. This shows that identical residual assumptions are fulfilled. Figure 1. Identical Residual Vs Fits Test 3.3.2. Normal Distribution Test Figure 2 shows the results of the Kolmogorov-Smirnov (KS) statistic for the normal distribution test. The Kolmogorov-Smirnov statistical value is 0.136 less than the Kolmogorov statistical value of 0.210 means that the residual normality test has followed the normal distribution. The residual plot of response approaches a straight line, so it can be said that the error does not deviate from the normal distribution substance. If the response is not normally distributed, it can be due to the form of the regression function which is incorrect or inappropriate. With the three residual analyzes above, it can be concluded that the residual test is identical, independent and normally distributed. http://www.iaeme.com/IJCIET/index.asp 137 [email protected] Annisa Rahmatika, Hariyadi, Jauhar Fajrin Figure 2. Normal Distribution Test 3.4. Analysis of Response Surface Characteristics The running result of the response surface program produces two images in the form of a contour graph and graph surface as shown in Figure 3 and Figure 4 below: Figure 3. Plot Contour Figure 4. Plot Surface In Figure 3 each variation shows the range of the magnitude of the response produced. The maximum conditions for the plot above are in dark green with a compressive strength above 50 kg / cm2. This color range will outline the direction of the optimum variable point. Determination of the optimum conditions of the above factors is proofed by the form of a threedimensional curve that procedures the optimum peak as shown in Figure 8. The plot surface image in Figure 8 displays the contour plot in three dimensions. In the picture above, optimum compressive strength is between level 0 and 1 addition of silica fume and cement. 3.5. Optimization The optimization results in Minitab 17 by using response surface method are shown in Figure 5. The graph results show the proportions for each independent variable which produces the most optimum response variable. The variable Silica Fume is at the level of 0.0510, which is as much as 121.53 gr. The cement variable is at the level of 0.2888, which is 514.65 gr, and the sand variable is at the level of 0.0493, which is 1409.86gr. The results of this optimization show the optimum composition that can be obtained by mortar, with the addition of silica fume as much as 23.6%. http://www.iaeme.com/IJCIET/index.asp 138 [email protected] The Application of Response Surface Methods (RSM) to Study the Effect of Partial Portland Cement Replacement Using Silica Fume on the Properties of Mortar Figure 5. Optimum Plot The result of this response surface optimization method is then re-tested to find out the quality confirmation design produced. This confirmation design was made with three samples with material composition based on the optimization results. This confirmation design was also carried out on testing the absorption and pH, which was in the form of analyzing the physical and mechanical properties of the mortar. 3.6. Compressive Test Confirmation Results The results of testing the mortar mixture with 23.6% silica fume obtained from the optimum plot were then compared with mortar without silica fume content. Mortar without added silica fume ingredients has a compressive strength of 25.6 MPa. The value of compressive strength on the confirmation mortar optimization results increased to reach 55.8 MPa. The value is shown in Figure 6. Figure 6. Comparison of Mortar testing result 3.7. Water Absorption Test Results Water absorption test of mortar is done by soaking the 56 days old specimen in water for 24 hours then the surface is dried awaiting no more water drips and then weighs the weight. Then the tested object is put into an oven with a temperature of 1100 for 24 hours then weighed again. Figure 6 shows a comparison of the mortar without silica fume with an optimized mortar by adding 23.6% silica fume. Mortar resulted from response surface methods optimization, can reduce water absorption by up to 5.43% compared to 8.84% absorptive silica mixtures. The results of 56 day mortar optimization can be seen in Table 6. http://www.iaeme.com/IJCIET/index.asp 139 [email protected] Annisa Rahmatika, Hariyadi, Jauhar Fajrin Table 5. Results of Absorption Test on Mortar N o 1 2 3 4 5 6 Silica Fume (gr) 0 0 0 121.53 121.53 121.53 Cement (gr) 600 600 600 514.66 514.66 514.66 SSD : Saturated Surface Dry Sand (gr) 1400 1400 1400 1409.86 1409.86 1409.86 SSD (gr) 306.53 311.75 294.24 299.7 297.56 293.75 SD (gr) 279.34 283.99 268.44 285.89 281.23 275.48 SD : Surface Dry WA (%) 8.87 8.905 8.768 4.608 5.488 6.22 Average WA (%) 8.848 5.438 WA : Water Absorption 3.8. Mortar pH Test Results The pH test on mortar without silica fume additives compared with mortar with the addition of the optimized silica fume can be seen in Figure 7. The pH test results showed that the mortar without silica fume had a pH of 9.63, whereas with the addition of silica fume, the optimization results in pH 9.75. Addition of silica fume as a substitute material for cement in mortar can maintain pH. The mortar remains alkaline according to the provisions of the pH of the mortar, which is> 9, so the function of the mortar to protect the reinforcement inside it from destructive acid is remain intact. Figure 7. pH Comparison of Mortar 4. CONCLUSION The primary conclusion drawn was that the method used in this study has demonstrated the inferential results of an experimental work in civil engineering field. More specific outcomes are outlined as follows: 1) The results of analysis with Response surface method produce, the optimum proportion of mortar is obtained by the composition of silica fume : cement : sand, which is 121.53 gr : 514.65 gr : 1409.8 gr. The results of testing the optimal confirmation test obtained compressive strength of 55.8 MPa, higher than the mortar compressive strength without silica which is 25.6 MPa. 2) Adding 23.6% of the silica-fume material from the optimum composition, is able to optimize the mortar mixture to be more waterproof. This is known from the decrease in water absorption on mortar up to 5.43% compared to mortar without silica which absorbs up to 8.48% water 3) The results of pH testing to the mortar with additional silica fume material showed that the mortar remained in an alkaline state (> 9). http://www.iaeme.com/IJCIET/index.asp 140 [email protected] The Application of Response Surface Methods (RSM) to Study the Effect of Partial Portland Cement Replacement Using Silica Fume on the Properties of Mortar REFERENCES [1] Samekto, W., Rahmadiyanto, C. Concrete Technology, Kanisius, ISBN: 979-672-5649, Yogyakarta, 2001. (in Indonesian) [2] American Concrete Institute Committee 234. Guide for the Use of Silica Fume in Concrete. Detroit : American Concrete Institute, 1996. [3] Mohamed, H. A, Effect of fly ash and silica fume on compressive strength of selfcompacting concrete under different curing conditions, Ain Shams Engineering Journal, 2(2), 79-86, 2011. [4] Amudhavalli, N.K., Mathew, J. Effect of Silica Fume on Strength and Durability Parameters of Concrete. International Journal of Engineering Sciences & Emerging Technologies, Vol 3,Issue 1, 2012, pp. 28-35. [5] Sundravel K, Vijaya., Aruldasu, K., Vijayasrinivasan,K. Experimental study on strength characteristics of Geopolymer concrete using Silica fume, Journal: IJERM, Vol 02,Issue11,November 2015, pp no: 57-60. [6] Dewi, A.K., Sumarjaya, I.W., Srinadi, I.G.A.M. Application of Surface Response Methods in Optimization Problems, Vol 2 , 2013, (2): 32-36. (in Indonesian) [7] Fajrin, J., Pathurahman, and Pratama L.G. Application of Analysis of Variance (ANOVA) Method to Assess the Effect of Addition of Silica Fume to Physical and Mechanical Properties of Mortar, Jurnal Rekayasa Sipil (JRS-Unand),. 12(1): p. 11-23, 2016. (in Indonesian) [8] SNI 03-6882-2002, Mortar Specifications for Wall Work, 2002. (in Indonesian) [9] SNI 03-6825-2002, Test Method of Compressive Strength of Portland Cement Mortar for Civil Works, 2002. (in Indonesian) [10] SNI 2493-2011, Procedures for Making and Maintenance of Concrete Test Samples in the Laboratory, 2011. (in Indonesian) http://www.iaeme.com/IJCIET/index.asp 141 [email protected]